... of Technology, Gokiso-cho, Showa-ku, Nagoya, Aichi 466-8555, Japan ...... S.; Nitta , K.; Inazawa , S. Intermediate-temperature ionic liquid NaFSA-KFSA and ...
Jun 12, 2017 - Frontier Research Institute for Materials Science (FRIMS), Nagoya Institute of Technology, Gokiso-cho, Showa-ku, Nagoya, Aichi 466-8555, Japan. Â§ Mi2i/GREEN, National Institute of Materials Science (NIMS), 1-2-1, Sengen, Tsukuba, Ibar
Jun 12, 2017 - Frontier Research Institute for Materials Science (FRIMS), Nagoya Institute of Technology, Gokiso-cho, Showa-ku, Nagoya, Aichi 466-8555, Japan. Â§ Mi2i/GREEN, National Institute of Materials Science (NIMS), 1-2-1, Sengen, Tsukuba, Ibar
Jul 22, 2017 - Department of Applied Chemistry, Tokyo Denki University, 5 Senju Asahi-Cho, Adachi, Tokyo 120-8551, Japan. Chem. Mater. , 2017, 29 (16), ...
Available reversible capacities are possibly increased into 300 mAh g-1 (1,000 mWh g-1 vs. Li metal). Page 3 of 34. ACS Paragon Plus Environment. Chemistry ...
Jun 12, 2017 - Department of Applied Chemistry, Tokyo Denki University, 5 Senju Asahi-Cho, Adachi, Tokyo 120-8551, Japan. â¡. Frontier Research Institute ...
Jul 22, 2017 - Moreover, the electrode performance of the sample is limited by the nanosize phase segregation in the single particles. The heat-treatment ...
Jun 12, 2017 - candidate,2 but the limited energy density of positive/negative electrodes ... Although the size of Na+ is much larger than those of ... These rings ... of 0 â¤ x â¤ 0.38, where MnâO hybridized bands are mainly .... spectra of Na1.
Jul 22, 2017 - The as-prepared sample was mixed with acetylene black (sample: AB = 90:10 in wt ...... Structural and mechanistic revelations on high capacity ...
NaFeO2 structure requires the simultaneous use of a specific precursor (Î²-NaFeO2 and not Î±-. NaFeO2), a reducing agent (carbon), and mechanical milling, ...
Subscriber access provided by UNIV AUTONOMA DE COAHUILA UADEC
Oxygen activity in Li-rich disordered rock-salt oxide and influence of LiNbO surface modification on the electrochemical performance 3
Musa Ali Cambaz, Bhaghavathi P. Vinayan, Holger Geßwein, Alexander Schiele, Angelina Sarapulova, Thomas Diemant, Andrey Mazilkin, Torsten Brezesinski, R. Jürgen Behm, Helmut Ehrenberg, and Maximilian Fichtner Chem. Mater., Just Accepted Manuscript • Publication Date (Web): 22 May 2019 Downloaded from http://pubs.acs.org on May 29, 2019
Just Accepted “Just Accepted” manuscripts have been peer-reviewed and accepted for publication. They are posted online prior to technical editing, formatting for publication and author proofing. The American Chemical Society provides “Just Accepted” as a service to the research community to expedite the dissemination of scientific material as soon as possible after acceptance. “Just Accepted” manuscripts appear in full in PDF format accompanied by an HTML abstract. “Just Accepted” manuscripts have been fully peer reviewed, but should not be considered the official version of record. They are citable by the Digital Object Identifier (DOI®). “Just Accepted” is an optional service offered to authors. Therefore, the “Just Accepted” Web site may not include all articles that will be published in the journal. After a manuscript is technically edited and formatted, it will be removed from the “Just Accepted” Web site and published as an ASAP article. Note that technical editing may introduce minor changes to the manuscript text and/or graphics which could affect content, and all legal disclaimers and ethical guidelines that apply to the journal pertain. ACS cannot be held responsible for errors or consequences arising from the use of information contained in these “Just Accepted” manuscripts.
Oxygen activity in Li-rich disordered rock-salt oxide and influence of LiNbO3 surface modification on the electrochemical performance
Musa Ali Cambaz1, Bhaghavathi P. Vinayan1, Holger Geßwein2, Alexander Schiele3, Angelina Sarapuolva2, Thomas Diemant4, Andrey Mazilkin3,5, Torsten Brezesinski3, R. Jürgen Behm1,4, Helmut Ehrenberg1,2, Maximilian Fichtner*1,3
Abstract Li-rich disordered rock-salt oxides such as Li1.2Ni1/3Ti1/3Mo2/15O2 are receiving increasing attention as high-capacity cathodes due to their potential as high-energy materials with variable elemental composition. However, the first-cycle oxygen release lowers the cycling performance due to cation densification and structural reconstruction on the surface region. This work explores the influence of lithium excess on the charge compensation mechanism and the effect of surface modification with LiNbO3 on the cycling performance. Moving from a stoichiometric LiNi0.5Ti0.5O2 composition towards Li-rich Li1.2Ni1/3Ti1/3Mo2/15O2, oxygen redox is accompanied by oxygen release Thereby, cationic charge-compensation is governed by the Ni2+/3+ and Mo3+/6+ redox reaction. Contrary to the bulk oxidation state of Mo6+ in the charged state, a mixed Mo valence on the surface is found by XPS. Furthermore, it is observed that smaller particle sizes result in higher specific capacities. Tailoring the surface properties of Li1.2Ni1/3Ti1/3Mo2/15O2 by a solid electrolyte layer of LiNbO3 altered the voltage profile, resulting in a higher average discharge voltage as compared to the unmodified material. The results hint at the inter-diffusion of cations from the metal oxide surface coating into the electrode material leading to bulk composition changes (doping) and segregated Nb-rich surface. The main finding of this work is the enhanced cycling stability and lower impedance of the surface modified compound. We argue that surface densification is mitigated by the Nb doping/surface modification.
Introduction The development of lithium-ion batteries (LIBs) with high energy density is one of the primary objectives in the energy storage field. The cathode material is considered as the bottleneck for improving the energy density. Conventional layered oxides like LiCoO2 and LiNi1/3Mn1/3Co1/3O2 exhibit stable specific capacities between 145–165 mAh g-1.1–3 Therefore, Li-rich layered oxides xLi2MnO3.(1−x)LiMO2 (M=3d transition metals), which promise higher capacities are now pursued as future cathode materials.4,5 These compounds offer specific capacities exceeding 200 mAh g-1, which results from the fact that charge can be stored on both the transition metal (Tm) cation and the oxygen anion.6–9 All of these materials have ordered structures. Li-rich disordered rock-salt oxides (DRS) with α-LiFeO2-type structure lately attracted considerable attention. Even though lithium migration is hindered in cation-disordered rock-salt oxides, they can in principle function well as high-capacity cathode materials. For a threshold ratio lithium: transition metal (Li:Tm) ≥ 1.09, the lithium sites can percolate sufficiently within the structure and form favorable diffusion pathways.10,11 Recently, Yabuuchi et al.12,13 demonstrated that for Li-rich cation-disordered Li3NbO4-MeO (M=Fe, Ni, Mn), a significant portion of the charge comes from reversible oxygen redox and is not mainly due to oxygen release. Oxygen redox can be beneficial, as it contributes to the capacity in the high-voltage range. However, too much oxidation seems to be detrimental, as oxygen loss can be triggered. This leads to a near-surface cation-densification, which can severely impede the Li diffusion.14 The generation of highly reactive oxygen radicals (in the form of O2-/O- or O2-2 in the bulk of the material) or even oxygen vacancies (after oxygenloss) on the particle surface during the electrochemical process is presumed to result in the formation of a resistive surface layer due to electrolyte decomposition and structural transformation.15–17 Thus, strategies to stabilize the particle surface to alleviate or even overcome these problems are needed to improve the performance of Li-rich disordered rocksalt oxides. 3 ACS Paragon Plus Environment
Li1.2Ni1/3Ti1/3Mo2/15O2 is a promising cathode material, which exhibits high specific capacities, but suffers from oxygen release.10,18Here, we propose a surface modification strategy using LiNbO3 in order to reduce the surface degradation and improve the electrochemical performance.19,20
Result & Discussion Synthesis & Characterization We chose to investigate a solid-solution between the stoichiometric cation-disordered Fm-3m Li2NiTiO4
(Li1.6Mo0.4O2), targeting lithium-rich cation-disordered Li-Ni-Ti-Mo oxide. For a clear representation of the lithium-to-transition metal ratio, we use the notation LiMO2. LiNi0.5Ti0.5O2 is adopting an α-LiFeO2-type crystal structure, where Li and the transition metals share the same octahedral site and are randomly distributed without any long-range order. These types of compounds are referred to as cation-disordered rock-salt oxides in the literature.21 Depending on the degree of the random occupation (from partial to full occupancy), the extent of cation-disorder varies. For the cation-ordered triclinic P-1 Li4MoO5, Mo+6 ions occupy the octahedral sites in a cubic close-packed (ccp) anion lattice with Li+ occupying the remaining octahedral sites. The structure is built up of [Mo2O10] clusters, consisting of edge-sharing MoO6 octahedra.22,23 The hypothetical binary mixture between “Li4MoO5-Li2NiTiO4” forms a single-phase solid-solution with Li1.2Ni1/3Ti1/3Mo2/15O2 stoichiometry and crystallizes in the α-LiFeO2-type structure as illustrated in Figure 1a. Li1.2Ni1/3Ti1/3Mo2/15O2 has been synthesized and subsequently coated with 5 wt. % LiNbO3 on the pristine powder (see experimental details below). No evidence of the presence of a LiNbO3 phase was found in the diffraction data of the LiNbO3-coated Li1.2Ni1/3Ti1/3Mo2/15O2. It has been shown that the metal oxide coating can react with the bulk material under hightemperature treatment.24,25 This leads to niobium substitution in this specific case. In the 4 ACS Paragon Plus Environment
following, LiNi0.5Ti0.5O2 is referred to as LNT-0, Li1.2Ni1/3Ti1/3Mo2/15O2 as LNTM-20 and LiNbO3-coated Li1.2Ni1/3Ti1/3Mo2/15O2 as Nb-LNTM-20. The number at the end of the abbreviation indicates the lithium excess. Rietveld refinement analysis of LNT-0, LNTM-20, and Nb-LNTM-20 is shown in Figure S1a,b,c. The refined lattice parameter for a singlephase fit in Fm-3m space group is: a = 4.141830(21) Å for LNT-0, a = 4.146881(33) Å for LNTM-20 and a = 4.146980(24) Å for Nb-LNTM-20. Nb-LNTM-20 shows a slightly larger a-lattice parameter, which is consistent with the larger cation radius of Nb5+, compared to Ni2+ and Ti4+. The chemical composition of compounds has been determined by inductively coupled plasma optical emission spectroscopy (ICP-OES) and is given in Table S1. Transmission electron microscopy (TEM) images are shown in Figure S2, depicting small spherical crystallites around 100 nm in diameter for LNT-0 and LNTM-20. For more insight into the coating, dark-field scanning transmission electron microscopy-energy dispersive Xray spectroscopy (STEM-EDX) mapping of Nb-LNTM-20 was carried out. The corresponding maps of Ni, Ti, Mo, and Nb are shown in Figure 1b,c. The Nb signal was found throughout the particle, with an increasing intensity from the center towards the edge. This indicates some Nb segregation to the outer surface. The combined X-ray diffraction (XRD) and STEM-EDX data suggest partial incorporation of Nb into the Li-Ni-Ti-Mo bulk lattice. A line scan along a crystallite grain confirms a Nb-rich outer surface layer of varying thickness (up to 12 nm). We estimate that ~47% of the Nb is substituted into the phase, leading to a nominal stoichiometry of LixNi0.328Ti0.328Mo0.131Nb0.016O2. X-ray photoelectron spectroscopy (XPS) results in Figure S3 indicate that Nb is in the +5 oxidation state.
Figure 1: a) XRD pattern of LiNi1/2Ti1/2O2 (LNT-0), Li1.2Ni1.3Ti1/3Mo2/15O2 (LNTM-20), LiNbO3-coated Li1.2Ni1/3Ti1/3Mo2/15O2 (Nb-LNTM-20) and Li4MoO5, b) TEM image of NbLNTM-20 and c) STEM-EDX mapping results obtained on Nb-LNTM-20 and line profile for the Nb-L edge.
Electrochemical Properties The
measurements. Figure 2a shows the charge-discharge profiles for LNT-0, LNTM-20, and NbLNTM-20 half-cells. The samples were cycled in the voltage range of 4.5-1.5 V vs. Li+/Li 6 ACS Paragon Plus Environment
using a constant specific current of 20 mA g-1. The specific discharge capacity increased significantly from 100 mAh g-1 to 220 mAh g- 1 changing from stoichiometric LNT-0 to Lirich LNTM-20. This increase in accessible capacity agrees with expectations based on percolation theory.10,11,26 The latter predicts that the 0-TM site can percolate and form extended lithium networks with 9% excess lithium, thus allowing more lithium to be intercalated / deintercalated. For Nb-LNTM-20, the voltage profile changed compared to the pristine sample. This is obvious from the corresponding differential capacity curves. Remarkably, Nb-LNTM-20 showed a longer and more defined upper voltage plateau and higher capacity contribution in the high-voltage regime > 2.5 V than LNTM-20. LNTM-20 showed an overall higher initial specific discharge capacity. However, a significantly higher fraction of the capacity is gained in the low-voltage regime (< 2.5 V), accompanied by a lowvoltage plateau around 2.1 V. In order to assess the influence of particle size on the accessible specific capacity, the sintering time was varied. The average particle sizes of LNTM-20 sintered for 2h and 4h and Nb-LNTM-20 sintered for 4h were 96, 220 and 176 nm, respectively, as shown in Figure S4a-c. LNTM-20 with an average particle size of 220 nm displayed a much lower specific discharge capacity of 170 mAh g-1 as compared to LNTM-20 with an average size of 96 nm (Figure S5), indicating a particle size dependence of the accessible capacity. This points to diffusion limitations. Figure 2b illustrates the rate performance of all compounds, which involved five consecutive cycles at a constant specific current. At higher currents, Nb-LNTM-20 retained more of the capacity than both LNT-0 and LNTM-20. For specific currents of 20, 50, 100, 200, 400 mA g-1, Nb-LNTM-20 exhibited specific capacities of 200, 174, 157, 135, 108 mAh g-1, whereas for LNTM-20 the corresponding values were 220, 164, 137, 115, 95 mAh g-1. For specific currents >50 mA g-1, Nb-LNTM-20 showed higher discharge capacities. The respective first cycle charge-discharge profiles for each current step are shown for both LNTM-20 and Nb-LNTM-20 in Figure 2c,d. For higher currents, we observed an increase in polarization and a decrease in the specific 7 ACS Paragon Plus Environment
capacity. Figure 2e shows the cycling stability of the investigated electrode materials. NbLNTM-20 demonstrated better capacity retention compared with LNTM-20. The better rate capability, in conjunction with the improved cycling stability, further highlights the importance of surface modification. Low capacity retention for Li-rich rock-salt oxides is a widely observed phenomenon.8,27,28 It is believed to originate from the participation of anions in the charge-compensation process (oxygen redox/release) as discussed below. Note that the charge-discharge profiles for Nb-LNTM-20 in the later cycles reveal the appearance of a lowvoltage plateau and the voltage profile resembles the behavior of LNTM-20, as shown in Figure 2f. With prolonged cycling, the voltage hysteresis increased along with an increased capacity contribution from the low-voltage region <2.5 V. Furthermore, the cycling stability of LNTM-20 appears to depend on the charge cut-off voltage, showing severe degradation when charged to high potentials. Being charged to high potentials, the Li-rich DRS can exhibit irreversible phenomena like oxygen evolution from the surface and side reactions.27 The first-cycle oxygen release for LNTM-20 is believed to cause cation-densification and structural reconstruction of the surface phase, thereby impeding Li conductivity and leading to impedance build-up. The observed plateau around 2.2 V has been related to surface densification after oxygen loss.18,29 For Nb-LNTW-20, this plateau is greatly reduced. Thus, surface modification seems to be beneficial in protecting the reactive surface and impeding surface densification.30 For a relatively narrow voltage window of 4.1-2.0 V, oxygen evolution or oxygen participation can be suppressed, and better cycling stability is achieved. This will be discussed in the following sections. Cycling LNTM-20 in a smaller voltage window leads to more symmetric profiles with lower voltage hysteresis as shown in Figure S6. Nb-LNTM-20 was subjected to milling in organic solvent and sintering as additional processing steps, which may affect its electrochemistry. In order to elucidate the influence of such additional steps on the electrochemistry, LNTM-20 was processed in the same way, without the addition of lithium and niobium precursors. The resulting charge-discharge profile 8 ACS Paragon Plus Environment
is presented in Figure S7a and the rate capability test shown in Figure S7b. The processed LNTM-20 showed a slightly lower specific capacity and a larger hysteresis, possibly due to lithium leaching during the solvent treatment.
Figure 2: a) Charge-discharge profiles of LNT-0, LNTM-20 and Nb-LNTM-20 with the corresponding differential capacity plots of the discharge cycle at 20 mA g-1. b) Rate capability test for all compounds in the range of 4.5-1.5 V vs. Li+/Li. c) Voltage profiles of LNTM-20 and d) Nb-LNTM-20 for different specific currents. e) Cycling stability of all compounds for various cut-off voltages at 20 mA g-1. f) Charge-discharge profiles of LNTM20 (1st cycle) and Nb-LNTM-20 (1st and 26th cycles).
As mentioned above, we hypothesize that the surface phase evolution is indicated by the appearance of the low-voltage plateau ~ 2.2 V. For the modified compound the first discharge does not reveal any visible low voltage plateau but appears with higher cycle numbers as shown in Figure 2f. On the contrary, the unmodified sample shows already in the first discharge a visible low voltage plateau from which we inferred that the surface phase evolution is mitigated for the surface modified Nb-LNTM-20. Electrochemical impedance spectra were measured to gain a better understanding of the improved cycling performance. Figure 3 shows the AC impedance spectra (Nyquist plots) of pristine LNTM-20 and of surface-modified Nb-LNTM-20, measured after 2 and 40 cycles for the discharged state. The equivalent circuit31 is shown in the inset, and the fitting results are listed in Table S2. The spectra exhibit two semicircles at high and low frequencies, and a Warburg tail at very low frequencies. The first, potential independent semicircle is attributed to the surface processes, e.g., the resistance of Li+ migration through electrode surface films (surface film resistance R1). The second, potential dependent semicircle reflects the charge transfer (interfacial) resistance R2.32 The Warburg tail is ascribed to the diffusion of Li-ions into the electrode material (Warburg element). Both materials (bare and Nb-coated) show a similar starting behavior and display growth in impedance after completion of the electrochemical cycling. The charge transfer resistances ‘R2’ of the pristine and surface-modified cathode after the 2nd and 40th cycles have been compared. R2is 20.3 and 67 Ω for the pristine cathode, and 7.7 and 23.2 Ω for the surface-modified compound, respectively. During prolonged cycling, the charge-transfer resistance significantly increases for the pristine cathode (by 43.7 Ω vs. 15.5 Ω for the surface-modified cathode). The increase in charge transfer resistance is tentatively attributed to structural changes on the surface. These results demonstrate that the surfacemodified compound shows a relatively low impedance after oxygen loss as compared to bare material. However, the increase in impedance with cycling is significant in accordance with the continuing capacity fading seen for Nb-LNTM-20. 10 ACS Paragon Plus Environment
Figure 3: Impedance spectra obtained for the discharged state (1.5 V) after the 2nd and 40th cycles, respectively on a) LNTM-20 and b) Nb-LNTM-20. The corresponding equivalent circuit is shown in the inset.
The electrode kinetics depend on both the ion transport and electronic conductivity and can limit the overall performance. The total conductivity of LNT-0 and LNTM-20 was studied by AC impedance spectroscopy at various temperatures as shown in Figure S8 and S9 in the SI. The activation energy (Ea) was calculated via Arrhenius equation, from the slope of ln (σ) vs. T−1, where σ is the conductivity and T represents the absolute temperature. LNTM-20 shows a 11 ACS Paragon Plus Environment
higher room temperature conductivity of ~3.0 × 10-6 S cm-1 compared to LNT-0 (~7.1 × 10-8 S cm-1). The donation of d-electrons can explain the increase in conductivity for LNTM-20 from Mo to the conduction band. The activation energy (Ea) for LNT-0 (319±19 meV) is higher than for LNTM-20 (249±16 meV). Overall, the conductivity is sufficiently high so that no electronic limitations are to be expected. Important to mention is that with the state of charge and the number of cycles the conductivity can vary by several orders of magnitude.33 For lithium-rich materials, both oxygen redox and lattice oxygen loss upon cycling are well-known phenomena.34,35 In order to find out whether oxygen release takes place in the case of overlithiated LNTM-20, in-situ differential electrochemical mass spectrometry (DEMS) measurements were conducted and the results compared to LNT-0, which served as reference material. To this end, half-cells were charged at C/10 to 4.5 V (1C = 210 mA g-1 for LNTM-20 and 100 mA g-1 for LNT-0) while monitoring gas evolution. As depicted in Figure 4 and S10, the LNTM-20 and LNT-0 half-cells showed first cycle charge capacities of 157 and 88 mAh g- 1. The specific capacities were lower for the thicker electrodes used in the DEMS measurements. CO2 evolution was observed, starting around 3.9 V for LNTM-20 and 4.1 V for LNT-0. The quantities detected for LNTM-20 were below 2 ppm up to 4.1 V (50 mAh g-1), thus making a precise determination of the onset potential difficult. As expected, significant oxygen release was only observed for the overlithiated material, starting at around 4.4 V. This is indicative of lattice changes during cycling operation, eventually leading to an oxygen-deficient (surface) structure. Chemical reactions of released oxygen with the electrolyte are not the only source of CO2 evolution, as both materials show similar behavior. Electrochemical electrolyte oxidation36,37 and decomposition of residual carbonate38,39 species from the synthesis, for instance, may also account for the CO2 evolution.
Figure 4: DEMS measurements of the first charge cycle at C/10 to 4.5 V for LNTM-20 half-cells. The cell voltage (black) is shown together with the O2 (blue) and CO2 (red) evolution.
Structural Changes upon Cycling In-situ XRD measurements were carried out to investigate the structural changes of LNTM-20 during two consecutive cycles between 4.5 and 1.5 V at C/30. The voltage profile and the changes in the a-lattice parameter from single-phase XRD refinement are shown in Figure 5, with an enlarged section displaying the pattern around the 002 reflection. During the 1st charge, three regimes can be seen. The first charge regime until 4 V reveals a sloped voltage profile, where the a-lattice parameter is continuously decreasing, thus reflecting lattice contraction. This finding can be associated with a Ni+2/+3 oxidation process [Ni+2 (r = 0.69 Å) and Ni+3 (r = 0.56 Å)]. The second regime is along the 4.3 V plateau, where the lattice parameter changes only slightly, and the third regime occurs towards the end of the charge, where the lattice parameter is continuously decreasing. This result can be attributed to oxygen oxidation and then release. In the mid regime, the lattice parameter is only changing in the beginning and at the end of charge. We argue that oxygen (O2-) oxidation is associated with a shrinkage of the oxygen framework because of the smaller size of the oxygen anion or due to the formation of peroxo-like species with shorter oxygen-oxygen bonds.40 During the 1st discharge, the lattice parameter continuously increases (lattice expansion) until 2.2 V. Further 13 ACS Paragon Plus Environment
discharge affects the lattice only slightly. During the second cycle upon discharge, a more pronounced plateau is observed for voltages <2.2 V, with only slight changes in the a-lattice parameter.
Figure 5: a) In-situ XRD pattern of LNTM-20 for two consecutive cycles in the range of 4.51.5 V at C/30. b) Corresponding voltage profile and changes in the a-lattice parameter from Rietveld refinement analysis. The red curves are the voltage profile and the red dots the measurement points, where the XRD patterns were collected.
Redox-Mechanism Further information on the redox mechanism of LNTM-20 and LNT-0 was obtained from X-ray absorption near-edge structure (XANES) measurements. Figure S11a shows the Ni K-edge spectra of pristine LNT-0 after charging to 4.5 V and then discharging to 1.5 V. Comparison of LNT-0 with a NiO reference compound reveals that the edge energy is similar indicating that the Ni oxidation state is +2. Figure 6a shows similar results for LNTM-20. During charge, the Ni K14 ACS Paragon Plus Environment
edge shifted significantly to higher energies, thereby reflecting an increase in oxidation state. Based on Faraday’s law, the theoretical capacities for different redox processes have been calculated and listed in Table 1. The oxidation state of Ti was determined by XPS to be +4, as shown in Figure S12. Ti+4 was fully oxidized and therefore assumed to be electrochemically inactive.41,42 Note that neither XANES nor XPS can rule out the formation of small amounts of Ti+3, in the atom percent range. The measured specific capacity for each state of charge can be used to estimate the average valence change. For LNT-0, the specific capacities for charging to 4.5 V and subsequently discharging to 1.5 V were 145 and 106 mAh g-1, respectively. This corresponds to 0.5 Li extraction and 0.37 Li intercalation per formula unit (f.u.), which can be attributed to the Ni+2/Ni+3 redox couple. Interestingly, LNTM-20 delivered 262 mAh g-1 during charge, corresponding to 0.86 Li per f.u., which is beyond the theoretical capacity for the Ni+2/+4 redox couple with 202 mAh g-1. This suggests that more redox active species are involved in the reaction, although electrolyte/electrode side reactions can also be expected. As confirmed by DEMS, O2 evolution takes place during charge and therefore, oxidation of O2- must be considered as an additional mechanism for charge compensation. For the consecutive discharge to 1.5 V, LNTM-20 exhibited a specific discharge capacity of 212 mAh g-1, corresponding to 0.73 Li per f.u. Simultaneously, the Ni K-edge shifts back to lower energies pointing to nickel reduction. In Figure S11b, the comparison between the Ni K-edge of LNT-0 and LNTM-20 in the charged state shows similar edge energies, suggesting that Ni is in the oxidation state +3 in both cases. In conclusion, oxidation to Ni+4 can be excluded for LNTM-20, limiting the nickel redox contribution to Ni+2/+3. Interesting to note is that the preedge peak intensity of Mo increased significantly after the first charge and remained at a higher value after the discharge, which is shown in Figure 6b. This finding indicates an increased distortion of the Mo-O6 octahedra compared to the pristine state. The intensities for these transitions are very sensitive to the coordination environment and the symmetry of the metal 15 ACS Paragon Plus Environment
center. For centrosymmetric symmetry, the pre-edge is weak, as it is limited by a weak electric quadrupole intensity mechanism.43 This pre-edge structure is typically observed for α-MoO3 with Mo in the oxidation state +6. The increase in pre-edge peak, with the shift of the white line to higher energies, suggests oxidation of Mo upon charging.44 Based on the results of a linear combination fit, the initial bulk oxidation state of Mo is estimated to be +4.7 and increases to around +6 upon charging. During discharge, it decreases to +3.2. XANES in fluorescence mode is a method to probe the bulk and investigate the average oxidation state; however, it is not sensitive to changes in the surface or near surface range. As evidenced by DEMS, O2 release takes place. Therefore, XPS was used to characterize the surface oxidation state for the charged material as shown in Figure S12. Note that a mixed oxidation state with mainly +6 and a minority at +4 is found for Mo. The partial reduction of Mo at the surface is possibly promoted after the oxygen loss.45,46 We did not observe any changes in the oxidation state of Ti. By charge balancing, we can roughly estimate the oxygen redox contribution to the total (reversible) capacity. Based on the derived oxidation states, Mo contributes with 52 mAh g-1 to the total specific charge capacity, without any contribution of the fully oxidized Ti+4. Assuming that during charging Ni is oxidized to +3, the Ni+2/+3 redox reaction can account for 101 mAh g-1. The remaining charge capacity must be compensated by oxygen anions, with an estimated contribution of 109 mAh g-1 during the first charge cycle. The local environment of the Ni ions in LNT-0 and LNTM-20 was investigated by extended X-ray absorption fine structure (EXAFS) measurements. Figure S11c and 6c depict the Fourier transformed (FT) spectra of the Ni K-edge for different states of charge. The first coordination shell (Ni-O) reflects the contribution of oxygen, while the second one is related to back-scattering from Ni ions (Ni-Ni). The most notable change takes place in the first coordination shell during charge, indicating that the charge compensation results in lower Ni-O peak amplitude. Ni+3 in the low-spin state is expected to result in a Jahn-Teller distortion, which is increased by oxidation. This 16 ACS Paragon Plus Environment
leads to a decrease in the amplitude of the Ni-O peak.47 The shape of the first coordination shell reveals the existence of two Ni-O peaks, suggesting distorted octahedral coordination. In Figure 6c, the amplitude R decreases for the 1st charge due to the change in the coordination environment and completely recovers after the 1st discharge. In the case of LNT-0, in Figure S11c, the amplitude R for the 1st discharge increases compared to the pristine state, suggesting that the pristine material partially contains Ni+3, which is being reduced during the 1st discharge.
Figure 6: a) XANES Ni K-edge spectrum for LNTM-20 and b) Mo K-edge spectrum for LNTM20. c) FT-EXAFS of Ni. Table 1: Theoretical specific capacity for different valence changes and the specific lithium capacity of LNT-0 and LNTM-20. Compound
Discussion and Conclusions Li-rich cation-disordered rock-salt oxides have promising properties such as high capacity. Furthermore, they allow for a large number of element combinations, which can be favorable in terms of sustainability and cost. However, challenges have to be overcome in order to achieve viable systems. So far, extended cycling stability with little capacity fading has not been demonstrated yet. In addition, problems hindering practical applications like voltage hysteresis and poor rate capability still need to be addressed and resolved. With increasing lithium-excess, new redox processes—which include oxygen activity—can be expected. Disadvantages of this process are the associated oxygen release, leading to surface degradation, side reactions with the electrolyte, cation densification and overall performance degradation. In particular, higher resistances lead to lower rate capability. DEMS measurements provided clear evidence that O2 is released for Li-rich LNTM-20, but not for stoichiometric LNT-0. In order to alleviate the above-mentioned drawbacks, approaches comprising both structural and surface/interface modifications have been intensively studied.30,31 Recently, Lee et al.29 demonstrated that substitution of oxygen by fluorine could mitigate oxygen loss and improve the cycling stability of the lithium-rich Li-Ni-Ti-Mo-(O/F) system. The fluorine substitution is an effective way, which enables an introduction of lithium-excess in low-valent systems without the use of heavy high-valent charge compensators, which can 19 ACS Paragon Plus Environment
lower the specific capacity. Practically, this approach aims to increase the cationic redox capacity. Fluorine doping has been reported to mitigate oxygen loss, improve capacity retention and increase the average voltage in some examples.18,48 However, stronger interactions between lithium and fluorine and lithium migration into tetrahedral sites for a high state of charge imposes constraints to the accessible capacity.49 Another interesting approach has been shown by Y. Shin et al.50 could experimentally demonstrate that oxygen loss can be mitigated by low-level doping of heavy elements such as Ta, resulting in surface modification. The improvement has been rationalized the enhanced oxygenretention of Ta and a tendency of the heavy elements to segregate at the surface due to the larger ionic radii. Our approach targets the surface modification and physical protection through a ceramic coating in order to mitigate the surface phase evolution, which leads to performance degradation. Here, we propose an approach comprising a surface treatment with LiNbO3 in order to improve
Li1.2Ni0.333Ti0.333Mo0.133O2 showed a high specific capacity but displayed a significant polarization
Li1.2Ni0.333Ti0.333Mo0.133O2, on the other hand, showed less polarization, with a higher average discharge voltage and a significantly higher capacity contribution in the high-voltage regime (>3.5 V). We argue that the change of the voltage profile can be attributed to the formation of a Li-Ni-Ti-Mo-Nb solid-solution due to partial inter-diffusion of cations from the surface coating into the active material during sintering. This observation is reflected in the lower impedance growth of Nb-LNTW-20 during cycling. We suggest that the lower charge-transfer resistance and impedance increase for the surface-modified compound can be attributed to the mitigated surface densification. For further optimization, a uniform coating is required. In addition, the influence of sintering temperature on the inter-diffusion mentioned above 20 ACS Paragon Plus Environment
needs to be better understood. Alternatively, LiTaO3 is a possible candidate compound that could be used for the surface modification, since Ta doping in a disordered rock-salt has been shown to affect the surface chemistry due to segregate of the heavy element dopant on the surface, thereby mitigating oxygen loss.50 In summary, we have demonstrated that high delithiation of Li1.2Ni0.333Ti0.333Mo0.133O2 triggers oxygen release, resulting in substantial performance decay. The changes in oxidation state, bond distance and coordination environment for different states of charge are illustrated. XANES spectroscopy revealed that Ni is oxidized from +2 to +3. At the same time, Mo changes its oxidation state from the pristine state with +4.7 to around +6 in the charged state; it is reduced to +3.2 in the consecutive discharge cycle. Furthermore, an irreversible structural distortion of the Mo environment was observed upon cycling. XPS revealed that in the charged state, Mo has a mixed oxidation state on the surface, with predominantly +6 and +4. Thus, in the fully charged state, we estimate that 109 mAh g-1 (around 0.36 Li per formula unit) are charge-compensated by oxygen anion oxidation, triggering O2 evolution, accompanied by partial reduction of Mo to +4 near the surface. Moreover, a strong particle size dependence of the accessible discharge capacity indicates the necessity of using small-size material for achieving high specific capacities. To the best of our knowledge, this is the first time a surface modification using the solid-state electrolyte LiNbO3 has been tested for cation-disordered rock-salt oxides. The voltage hysteresis was significantly reduced for Nb-LNTM-20 over LNTM-20. This observation was reflected by the lower impedance and also relatively lower impedance build-up as compared to pristine material. Overall, we conclude that surface modifications hold promise to further improve the rate capability and cycling performance of Li-rich cation-disordered rock-salt oxides.
Supporting Information 21 ACS Paragon Plus Environment
Rietveld refinement of LNT-0, LNTM-20, and Nb-LNTM-20. TEM images of LNT-0 and LNTM-20. The particle size distribution of Nb-LNTM-20 and LNTM-20 for different sintering times. Further electrochemical data for varying potential ranges, influence of solvent treatment and particle size. Nyquist and Arrhenius plots for LNT-0 and LNTM-20. XANES, EXAFS, and DEMS for LNT-0. XPS spectra of pristine and charged Nb-LNTM-20 and LNTM-20. Tabulated data for EIS fitting and ICP-OES atomic ratio.
Acknowledgments Financial support by the FET-OPEN project “LiRichFCC” of the European Commission (grant agreement #711792) is gratefully acknowledged. This work contributes to the research performed at CELEST (Center for Electrochemical Energy Storage Ulm-Karlsruhe). We want to thank Dr. Edmund Welter from Experiments Division XAS in PETRA III, Hamburg.
Experimental Section Synthesis: The procedure to synthesize LiNi0.5Ti0.5O2 and Li1.2Ni1/3Ti1/3Mo2/15O2 was adopted from Jinhyuk-Lee et al.29 Li4MoO5 was synthesized using modified conditions. Li2CO3 (Alfa Aesar, >99%), NiCO3 (Alfa Aesar, 99%), TiO2 nanopowder (<50 nm particle size, Alfa Aesar, 99.7%), and MoO2 (Alfa Aesar, 99%) were employed as the precursors. Other than for LiNi0.5Ti0.5O2, stoichiometric amounts of precursors were used. For Li1.2Ni1/3Ti1/3Mo2/15O2 and Li4MoO5, five % of excess Li was used. The precursors were ball milled for 24 h with 200 rpm using a Fritsch P6 planetary ball mill with 80 mL silicon nitride vial and silicon nitride balls, with a ball to powder weight ratio of 20:1. The mixture of the precursors was pelletized and then sintered at 750 °C for two h in air, followed by furnace cooling to 200 °C and immediate transfer inside an argon-filled glove box. Li4MoO5 was sintered at 900 °C for two h. After sintering, the pellets were manually ground into a fine powder.
For coating, we prepared a solution between solid lithium ethoxide (Sigma Aldrich, 95%) and liquid niobium isopropoxide solution (Alfa Aesar, 99%, ten wt% niobium isopropoxide in 50:50 (v:v) isopropanol/hexane) with a nominal stoichiometry of 1.05:1.0 of Li to Nb. Li1.2Ni1/3Ti1/3Mo2/15O2 was ball milled with the prepared coating solution using a Fritsch P9 with 15 mL vial volume for 12 h at 200 rpm (ball to powder ratio of 15:1). Subsequently, the mixture was dried overnight in an oven in an argon-filled glove box and then pelletized and sintered at 400 °C for two h in air, followed by furnace cooling to 200 °C and immediate transfer into an argon-filled glove box. After the sintering, the pellets were manually ground into a fine powder. Electrochemical Measurements: Electrochemical tests were carried out in Swagelok-type cell using lithium as the counter electrode. Electrode slurries were made of 90 wt. % composite and 10 wt. % polyvinylidene difluoride (PVDF) binder with N-methyl-2pyrrolidone (NMP) as the solvent. The composite consists of active material and Super C65 carbon black in a weight ratio of 80:20. The mixed slurry was coated on an aluminum foil using the doctor blade technique and dried at 120 °C for 12 h under vacuum. Each working electrode (12 mm diameter) contained about 3 mg of active material, and Li foil was used as the counter electrode. LP30 from BASF (ethylene carbonate/dimethyl carbonate, 1:1 weight ratio with 1M LiPF6) was used as the electrolyte. Temperature-controlled galvanostatic charge-discharge experiments were conducted at 25 °C in a climate chamber using an Arbin electrochemical workstation. Impedance spectroscopy (EIS): For a better understanding of the cycling performance of surface-modified Nb-LNTM-20 relative to pristine LNTM-20, electrochemical impedance spectra were measured at 25 °C after the 2nd and 40th cycles. Electrochemical impedance spectroscopy (EIS) was performed using a three-electrode PAT-Cell (EL-CELL, Germany) with a Li ring as the reference electrode and Li metal (18 mm) as the counter electrode. The 23 ACS Paragon Plus Environment
working electrode size was 18 mm, and aluminum served as the current collector. The experiments were conducted using a Bio-Logic electrochemical workstation with an applied sinusoidal excitation voltage of 10 mV in the frequency range between 200 kHz and 0.1 Hz. Differential electrochemical mass spectrometry: In-situ gas analysis was performed by use of differential electrochemical mass spectrometry (DEMS). The setup has been described elsewhere.37,51 Custom cells with gas in- and outlets were assembled in an argon-filled glove box. The cathodes used (40 mm diameter with a 4 mm hole for proper gas extraction) had areal loadings of about 1 mgLNT-0/cm2 and 1.6 mgLNTM-20/cm2. GF/A (42 mm diameter, GE Healthcare Life Sciences, Whatman) was used as the separator, 600 µL of LP47 (1M LiPF6 in ethylene carbonate/diethyl carbonate, 3:7 by weight, BASF SE) as the electrolyte, and 600 µm-thick Li metal foil (Albemarle Germany GmbH) with a diameter of 40 mm as the counter electrode. A constant carrier gas flow (2.5 mLHe/min, purity 6.0) was applied during DEMS measurements for gas extraction reason. The gas was analyzed via mass spectrometry (GSD 320, OmniStar Gas Analysis System, Pfeiffer Vacuum GmbH). After each run, a calibration gas of known composition was introduced to quantify the measured ion currents. Conductivity: To measure the conductivity, powder materials were pressed into pellets with a diameter of 8 mm and coated with a gold layer on both sides by sputtering. AC impedance data were collected in the frequency range from 0.1 Hz to 1 MHz (10 mVrms amplitude) using a frequency response analyzer (ZAHNER-Elektrik GmbH) at various temperatures (25-80 °C). After each temperature, the samples were allowed to equilibrate for a substantial amount of time. The impedance data were fitted and analyzed using the ZMAN 2 software. X-ray Absorption Spectroscopy: The P65 XAS beamline (PETRA III, Hamburg) provides a relatively large beam (0.51 mm²) and a moderate photon flux density. The 11 period miniundulator delivers a monochromatic photon flux of about 1011 ph/s. Two plane mirrors with variable angle of incidence and three different surface coatings are installed in front of the 24 ACS Paragon Plus Environment
water-cooled double crystal monochromator. Si (111) and Si(311) crystals are used for the energy ranges of 4-22 keV and 7-44 keV, respectively. The P65 beamline is also equipped with a 7 pixel HPGe energy dispersive detector and Si-PIPS diode. X-ray absorption spectroscopy measurements were performed in both transmission and fluorescence modes. For ex-situ measurements, the step-scan mode with a duration of about 10-11 min for each spectrum was used. The spectra were processed using the Demeter software package based on IFEFFIT and FEFF.52 X-ray diffraction: In-situ X-ray diffraction patterns were collected using modified coin cells on a parallel beam laboratory diffractometer with a microfocus rotating anode (Mo-Kα radiation) in transmission geometry and a Pilatus 300K-W area detector. The coin cells comprise an LNTM-20-based cathode, a Li metal anode and a Whatman glass fibre separator. 1M LiPF6 in ethylene carbonate: dimethyl carbonate 1:1 (w:w) from BASF served as the electrolyte. Galvanostatic charge-discharge cycling was performed with an Ivium potentiostat between 1.5 and 4.5 V at 10 mA g-1. Diffraction patterns were collected every 300 s. Two consecutive patterns were added up to eliminate cosmic spikes on the detector. The diffraction images were integrated using the pyFAI software53 and analyzed with the Rietveld method using TOPAS V6. X-ray photoelectron spectroscopy: The elemental composition of the surface region was analyzed by XPS using a Physical Electronics PHI 5800 ESCA system. The measurements were carried out with monochromatic Al-Ka radiation (250 W, 13 kV) at a detection angle of 45° and with pass energies of 93.9 and 29.35 eV for survey and detail measurements, respectively. An electron flood gun was used for sample neutralization. The main C 1s peak was set to 284.8 eV for binding energy calibration. Some samples were subject to Ar+ sputtering (sputter rate ~1 nm min-1, 1 mA, 5 kV) to remove the topmost surface layer.
Scrosati, B.; Hassoun, J.; Sun, Y.-K. Lithium-Ion Batteries. A Look into the Future. Energy Environ. Sci. 2011, 4 (9), 3287.
Myung, S.-T.; Maglia, F.; Park, K.-J.; Yoon, C. S.; Lamp, P.; Kim, S.-J.; Sun, Y.-K. Nickel-Rich Layered Cathode Materials for Automotive Lithium-Ion Batteries: Achievements and Perspectives. ACS Energy Lett. 2017, 2 (1), 196–223.
Etacheri, V.; Marom, R.; Elazari, R.; Salitra, G.; Aurbach, D. Challenges in the Development of Advanced Li-Ion Batteries: A Review. Energy Environ. Sci. 2011, 4 (9), 3243.
Sun, Y.-K.; Myung, S.-T.; Park, B.-C.; Prakash, J.; Belharouak, I.; Amine, K. HighEnergy Cathode Material for Long-Life and Safe Lithium Batteries. Nat. Mater. 2009, 8 (4), 320–324.
Hy, S.; Liu, H.; Zhang, M.; Qian, D.; Hwang, B.-J.; Meng, Y. S. Performance and Design Considerations for Lithium Excess Layered Oxide Positive Electrode Materials for Lithium Ion Batteries. Energy Environ. Sci. 2016, 9 (6), 1931–1954.
Lu, Z.; Dahn, J. R. Understanding the Anomalous Capacity of Li/Li[NixLi(1/3−2x/3)Mn(2/3−x/3)]O2 Cells Using In Situ X-Ray Diffraction and Electrochemical Studies. J. Electrochem. Soc. 2002, 149 (7), 815–822.
Koga, H.; Croguennec, L.; Menetrier, M.; Douhil, K.; Belin, S.; Bourgeois, L.; Suard, E.; Weill, F.; Delmas, C. Reversible Oxygen Participation to the Redox Processes Revealed for Li1.20Mn0.54Co0.13Ni0.13O2. J. Electrochem. Soc. 2013, 160 (6), 786–792.
Rozier, P.; Tarascon, J. M. Review—Li-Rich Layered Oxide Cathodes for NextGeneration Li-Ion Batteries: Chances and Challenges. J. Electrochem. Soc. 2015, 162 (14), A2490–A2499.
Lee, J.; Urban, A.; Li, X.; Su, D.; Hautier, G.; Ceder, G. Unlocking the Potential of Cation-Disordered Oxides for Rechargeable Lithium Batteries. Science (80-. ). 2014, 343 (6170), 519–522. 26 ACS Paragon Plus Environment
Urban, A.; Lee, J.; Ceder, G. The Configurational Space of Rocksalt-Type Oxides for High-Capacity Lithium Battery Electrodes. Adv. Energy Mater. 2014, 4 (13), 1400478.
Yabuuchi, N.; Takeuchi, M.; Nakayama, M.; Shiiba, H.; Ogawa, M.; Nakayama, K.; Ohta, T.; Endo, D.; Ozaki, T.; Inamasu, T.; et al. High-Capacity Electrode Materials for Rechargeable Lithium Batteries: Li3NbO4 -Based System with Cation-Disordered Rocksalt Structure. Proc. Natl. Acad. Sci. 2015, 112 (25), 7650–7655.
Yabuuchi, N.; Nakayama, M.; Takeuchi, M.; Komaba, S.; Hashimoto, Y.; Mukai, T.; Shiiba, H.; Sato, K.; Kobayashi, Y.; Nakao, A.; et al. Origin of Stabilization and Destabilization in Solid-State Redox Reaction of Oxide Ions for Lithium-Ion Batteries. Nat. Commun. 2016, 7, 13814.
Fell, C. R.; Qian, D.; Carroll, K. J.; Chi, M.; Jones, J. L.; Meng, Y. S. Correlation Between Oxygen Vacancy, Microstrain, and Cation Distribution in Lithium-Excess Layered Oxides During the First Electrochemical Cycle. Chem. Mater. 2013, 25 (9), 1621–1629.
Cabana, J.; Kwon, B. J.; Hu, L. Mechanisms of Degradation and Strategies for the Stabilization of Cathode–Electrolyte Interfaces in Li-Ion Batteries. Acc. Chem. Res. 2018, 51 (2), 299–308.
Xu, B.; Fell, C. R.; Chi, M.; Meng, Y. S. Identifying Surface Structural Changes in Layered Li-Excess Nickel Manganese Oxides in High Voltage Lithium Ion Batteries: A Joint Experimental and Theoretical Study. Energy Environ. Sci. 2011, 4 (6), 2223.
Qian, D.; Xu, B.; Chi, M.; Meng, Y. S. Uncovering the Roles of Oxygen Vacancies in Cation Migration in Lithium Excess Layered Oxides. Phys. Chem. Chem. Phys. 2014, 16 (28), 14665–14668.
Lee, J.; Papp, J. K.; Clément, R. J.; Sallis, S.; Kwon, D.-H.; Shi, T.; Yang, W.; McCloskey, B. D.; Ceder, G. Mitigating Oxygen Loss to Improve the Cycling Performance of High Capacity Cation-Disordered Cathode Materials. Nat. Commun. 2017, 8 (1), 981.
Kim, H.; Byun, D.; Chang, W.; Jung, H.-G.; Choi, W. A Nano-LiNbO3 Coating Layer and Diffusion-Induced Surface Control towards High-Performance 5 V Spinel Cathodes for Rechargeable Batteries. J. Mater. Chem. A 2017, 5 (47), 25077–25089.
Ohta, N.; Takada, K.; Sakaguchi, I.; Zhang, L.; Ma, R.; Fukuda, K.; Osada, M.; Sasaki, 27 ACS Paragon Plus Environment
T. LiNbO3-Coated LiCoO2 as Cathode Material for All Solid-State Lithium Secondary Batteries. Electrochem. commun. 2007, 9 (7), 1486–1490. (21)
Sebastian, L.; Gopalakrishnan, J. Li2MTiO4 (M=Mn, Fe, Co, Ni): New CationDisordered Rocksalt Oxides Exhibiting Oxidative Deintercalation of Lithium. Synthesis of an Ordered Li2NiTiO4. J. Solid State Chem. 2003, 172 (1), 171–177.
Hoffmann, R.; Hoppe, R. Two New Variants of the Sodium Chloride Type of Structure: On Lithium Molybdenum Oxide (Li4MoO5) and Lithium Tungsten Oxide (Li4WO5). Z. Anorg. Allg. Chem. 1989, 573, 157–159.
Yabuuchi, N.; Tahara, Y.; Komaba, S.; Kitada, S.; Kajiya, Y. Synthesis and Electrochemical Properties of Li4MoO5 –NiO Binary System as Positive Electrode Materials for Rechargeable Lithium Batteries. Chem. Mater. 2016, 28 (2), 416–419.
Appapillai, A. T.; Mansour, A. N.; Cho, J.; Shao-Horn, Y. Microstructure of LiCoO2 with and without “AlPO4” Nanoparticle Coating: Combined STEM and XPS Studies. Chem. Mater. 2007, 19 (23), 5748–5757.
Dahéron, L.; Dedryvère, R.; Martinez, H.; Flahaut, D.; Ménétrier, M.; Delmas, C.; Gonbeau, D. Possible Explanation for the Efficiency of Al-Based Coatings on LiCoO2: Surface Properties of LiCo1−xAlxO2 Solid Solution. Chem. Mater. 2009, 21 (23), 5607– 5616.
Glazier, S. L.; Li, J.; Zhou, J.; Bond, T.; Dahn, J. R. Characterization of Disordered Li(1+ x )Ti2xFe(1–3 x )O2 as Positive Electrode Materials in Li-Ion Batteries Using Percolation Theory. Chem. Mater. 2015, 27 (22), 7751–7756.
Twu, N.; Li, X.; Urban, A.; Balasubramanian, M.; Lee, J.; Liu, L.; Ceder, G. Designing New Lithium-Excess Cathode Materials from Percolation Theory: Nanohighways in Li x Ni 2–4 x /3 Sb x /3 O 2. Nano Lett. 2015, 15 (1), 596–602.
Koga, H.; Croguennec, L.; Ménétrier, M.; Mannessiez, P.; Weill, F.; Delmas, C. Different Oxygen Redox Participation for Bulk and Surface: A Possible Global Explanation for the Cycling Mechanism of Li1.20Mn0.54Co0.13Ni0.13O2. J. Power Sources 2013, 236, 250–258.
Lee, J.; Seo, D.-H.; Balasubramanian, M.; Twu, N.; Li, X.; Ceder, G. A New Class of High Capacity Cation-Disordered Oxides for Rechargeable Lithium Batteries: Li–Ni– Ti–Mo Oxides. Energy Environ. Sci. 2015, 8 (11), 3255–3265. 28 ACS Paragon Plus Environment
Chen, Z.; Qin, Y.; Amine, K.; Sun, Y.-K. Role of Surface Coating on Cathode Materials for Lithium-Ion Batteries. J. Mater. Chem. 2010, 20 (36), 7606.
Schipper, F.; Bouzaglo, H.; Dixit, M.; Erickson, E. M.; Weigel, T.; Talianker, M.; Grinblat, J.; Burstein, L.; Schmidt, M.; Lampert, J.; et al. From Surface ZrO2 Coating to Bulk Zr Doping by High Temperature Annealing of Nickel-Rich Lithiated Oxides and Their Enhanced Electrochemical Performance in Lithium Ion Batteries. Adv. Energy Mater. 2018, 8 (4), 1701682.
Aurbach Doron, Mikhail D. Levi, Elena Levi, Hanan Teller, Boris Markovsky, Gregory Salitra, Udo Heider, and L. H. Common Electroanalytical Behavior of Li Intercalation Processes into Graphite and Transition Metal Oxides. J. Electrochem. Soc. 1998, 145 (9), 3024–3034.
Amin, R.; Ravnsbæk, D. B.; Chiang, Y.-M. Characterization of Electronic and Ionic Transport in Li 1- x Ni 0 . 8 Co 0.15 Al 0.05 O 2 (NCA). J. Electrochem. Soc. 2015, 162 (7), A1163–A1169.
Twu, N.; Metzger, M.; Balasubramanian, M.; Marino, C.; Li, X.; Chen, H.; Gasteiger, H.; Ceder, G. Understanding the Origins of Higher Capacities at Faster Rates in Lithium-Excess LixNi2-4x/3Sbx/3O2. Chem. Mater. 2017, 29 (6), 2584–2593.
Strehle, B.; Kleiner, K.; Jung, R.; Chesneau, F.; Mendez, M.; Hubert, A. The Role of Oxygen Release from Li- and Mn-Rich Layered Oxides During the First Cycles Investigated by On-Line Electrochemical Mass Spectrometry. J. Electrochem. Soc. 2017, 164 (2), 400–406.
Metzger, M.; Strehle, B.; Solchenbach, S.; Gasteiger, H. A. Origin of H2 Evolution in LIBs: H2O Reduction vs. Electrolyte Oxidation. J. Electrochem. Soc. 2016, 163 (5), A798–A809.
Berkes, B. B.; Schiele, A.; Sommer, H.; Brezesinski, T.; Janek, J. On the Gassing Behavior of Lithium-Ion Batteries with NCM523 Cathodes. J. Solid State Electrochem. 2016, 20 (11), 2961–2967.
Renfrew, S. E.; McCloskey, B. D. Residual Lithium Carbonate Predominantly Accounts for First Cycle CO 2 and CO Outgassing of Li-Stoichiometric and Li-Rich Layered Transition-Metal Oxides. J. Am. Chem. Soc. 2017, 139 (49), 17853–17860.
Hatsukade, T.; Schiele, A.; Hartmann, P.; Brezesinski, T.; Janek, J. Origin of Carbon 29 ACS Paragon Plus Environment
Dioxide Evolved during Cycling of Nickel-Rich Layered NCM Cathodes. ACS Appl. Mater. Interfaces 2018, 10 (45), 38892–38899. (40)
Sathiya, M.; Rousse, G.; Ramesha, K.; Laisa, C. P.; Vezin, H.; Sougrati, M. T.; Doublet, M.-L.; Foix, D.; Gonbeau, D.; Walker, W.; et al. Reversible Anionic Redox Chemistry in High-Capacity Layered-Oxide Electrodes. Nat. Mater. 2013, 12 (9), 827– 835.
Tabuchi, M.; Nakashima, A.; Shigemura, H.; Ado, K.; Kobayashi, H.; Sakaebe, H.; Tatsumi, K.; Kageyama, H.; Nakamura, T.; Kanno, R. Fine Li(4 -x)/3Ti(2-2x)/3FexO2 (0.18 ≤x≤0.67) Powder with Cubic Rock-Salt Structure as a Positive Electrode Material for Rechargeable Lithium Batteries. J. Mater. Chem. 2003, 13 (7), 1747–1757.
Shigemura, H.; Tabuchi, M.; Sakaebe, H.; Kobayashi, H.; Kageyama, H. Lithium Extraction and Insertion Behavior of Nanocrystalline Li2TiO3-LiFeO2 Solid Solution with Cubic Rock Salt Structure. J. Electrochem. Soc. 2003, 150 (5), 638–644.
Yamamoto, T. Assignment of Pre-Edge Peaks in K-Edge x-Ray Absorption Spectra of 3d Transition Metal Compounds: Electric Dipole or Quadrupole? X-Ray Spectrom. 2008, 37 (6), 572–584.
Thackeray, M. M.; Kang, S.-H.; Johnson, C. S.; Vaughey, J. T.; Benedek, R.; Hackney, S. A. Li2MnO3-Stabilized LiMO2 (M = Mn, Ni, Co) Electrodes for Lithium-Ion Batteries. J. Mater. Chem. 2007, 17 (30), 3112–3125.
Lu, Z.; Dahn, J. R. Understanding the Anomalous Capacity of Li/Li[NixLi (1/3−2x/3)Mn(2/3−x/3)]O2 Cells Using In Situ X-Ray Diffraction and Electrochemical Studies. J. Electrochem. Soc. 2002, 149 (7), 815–822.
Deb, A.; Bergmann, U.; Cramer, S. P.; Cairns, E. J. Local Structure of LiNi0.5Mn0.5O2 Cathode Material Probed by in Situ x-Ray Absorption Spectroscopy. J. Appl. Phys. 2006, 99 (6), 063701.
Clément, R. J.; Kitchaev, D.; Lee, J.; Gerbrand Ceder. Short-Range Order and Unusual Modes of Nickel Redox in a Fluorine-Substituted Disordered Rocksalt Oxide LithiumIon Cathode. Chem. Mater. 2018, 30 (19), 6945–6956. 30 ACS Paragon Plus Environment
Kitchaev, D. A.; Lun, Z.; Richards, W. D.; Ji, H.; Clément, R. J.; Balasubramanian, M.; Kwon, D.-H.; Dai, K.; Papp, J. K.; Lei, T.; et al. Design Principles for High Transition Metal Capacity in Disordered Rocksalt Li-Ion Cathodes. Energy Environ. Sci. 2018, 11 (8), 2159–2171.
Shin, Y.; Kan, W. H.; Aykol, M.; Papp, J. K.; McCloskey, B. D.; Chen, G.; Persson, K. A. Alleviating Oxygen Evolution from Li-Excess Oxide Materials through TheoryGuided Surface Protection. Nat. Commun. 2018, 9 (1), 4597.
Berkes, B. B.; Jozwiuk, A.; Vračar, M.; Sommer, H.; Brezesinski, T.; Janek, J. Online Continuous Flow Differential Electrochemical Mass Spectrometry with a Realistic Battery Setup for High-Precision, Long- Term Cycling Tests. Anal. Chem. 2015, 87 (12), 5878 − 5883.
Ravel, B.; Newville, M. ATHENA , ARTEMIS , HEPHAESTUS : Data Analysis for X-Ray Absorption Spectroscopy Using IFEFFIT. J. Synchrotron Radiat. 2005, 12 (4), 537–541.
Ashiotis, G.; Deschildre, A.; Nawaz, Z.; Wright, J. P.; Karkoulis, D.; Picca, F. E.; Kieffer, J. The Fast Azimuthal Integration Python Library: PyFAI. J. Appl. Crystallogr. 2015, 48 (2), 510–519.